A Novel Antibacterial Dental Resin Composite
Yiming Weng1, Voon J. Chong1, Leah Howard1, Ruijie Huang2, Richard L. Gregory2, Dong Xie1* 1Department of Biomedical Engineering, Purdue School of Engineering and Technology, Indiana University-Purdue University at Indianapolis, Indianapolis, USA; 2Department of Oral Biology, School of Dentistry, Indiana University, Indianapolis, USA.
Received January 12th, 2012; revised February 20th, 2012; accepted March 10th, 2012
This study reports the synthesis and evaluation of a novel furanone-containing antibacterial resin composite. Compres-sive strength (CS) and S. mutans viability were used to evaluate the mechanical strength and antibacterial activity of the composites. With 5% to 30% addition of the furanone derivative, the composite showed no change in CS but a signifi-cant antibacterial activity with a 16% - 68% reduction in the S. mutans viability. Further, the antibacterial activity of the modified composite was not affected by human saliva. The aging study implies that the modified composite may have a long-lasting antibacterial function. Within the limitations of this study, it appears that this experimental resin composite may potentially be developed into a clinically attractive dental restorative due to its high mechanical strength and anti-bacterial function.
Keywords: Furanone Derivative; Antibacterial; Resin Composite; CS; S. mutans Viability
Long-lasting restoratives and restoration are clinically attractive because they can reduce patents’ pain and ex-pense as well as the number of their visits to dental of-fices [1-4]. In dentistry, both restorative materials and oral bacteria are believed to be responsible for the resto-ration failure . Secondary caries is found to be the main reason to the restoration failure of dental restora-tives including resin composites and glass-ionomer ce-ments [1-4]. Secondary caries that often occurs at the interface between the restoration and the cavity prepara-tion is primarily caused by demineralizaprepara-tion of tooth structure due to invasion of plaque bacteria (acid-pro- ducing bacteria) such as Streptococcus mutans (S. mu-tans) in the presence of fermentable carbohydrates . To make long-lasting restorations, the materials should be made antibacterial. Although numerous efforts have been made on improving antibacterial activities of dental restoratives, most of them have been focused on release or slow-release of various incorporated low molecular weight antibacterial agents such as antibiotics, zinc ions, silver ions, iodine and chlorhexidine [5-9]. Yet release or slow-release can lead or has led to a reduction of me-chanical properties of the restoratives over time, short- term effectiveness, and possible toxicity to surround- ing tissues if the dose or release is not properly con- trolled [5-9]. Materials containing quaternary ammonium
salt (QAS) or phosphonium salt groups have been stud-ied extensively as an important antimicrobial material and used for a variety of applications due to their potent antimicrobial activities [10-14]. These materials are found to be capable of killing bacteria that are resistant to other types of cationic antibacterials . The examples of the QAS-containing materials as antibacterials for dental restoratives include incorporation of a methacry-loyloxydodecyl pyridinium bromide as an antibacterial monomer into resin composites , use of methacry-loxylethyl cetyl ammonium chloride as a component for antibacterial bonding agents [16,17], and incorporation of quaternary ammonium polyethylenimine nanoparticles into resin composites [18,19]. All these studies found that the QAS-containing materials did exhibit significant antibacterial activities. However, our recent study found that incorporation of QAS into dental resin composites can significantly decrease mechanical strengths due to its strong hydrophilic characteristics, if the amount added is beyond a certain limit . In addition, it has been re-ported that human saliva can significantly reduce the antibacterial activity of the QAS-containing restoratives, probably due to electrostatic interactions between QAS and proteins in saliva [21-22]. Recently furanone deriva-tives have been found to have strong antitumor  and antibacterial functions . In the study, we would like to explore them in dental applications.
This paper reports the synthesis of a novel furanone derivative and the effect of this synthesized furanone
derivative on the antibacterial activity and compressive strength of the dental resin composite.
2. Materials and Methods
Bisphenol A glycerolate dimethacrylate (BisGMA), Bisphenol A ethoxylate dimethacrylate (BisEMA), ure-thane dimethacrylate (UDMA), triethylene glycol di-methacrylate (TEGDMA), dl-camphoroquinone (CQ), 2- (dimethylamino)ethyl methacrylate (DMAEMA), tolu- ene, acryloyl chloride (AC), 3,4-dichloromalealdehydic acid (DA), ethyl acetate and sodium bicarbonate were used as received from Sigma-Aldrich Co. (Milwaukee, WI) without further purifications. The untreated glass fillers from Herculite XRV (0.7 microns) were used as received from Sybron Dental Specialties (Newport Beach, CA).
2.2. Synthesis and Characterization
The new monomer, 5-acryloyloxy-3,4-dichlorocrotono- lactone (AD), was prepared from the reaction of 3,4- dichloromalealdehydic acid (DA) with acryloyl chloride (AC) in the presence of toluene at 90˚C - 100˚C for 3 - 4 h. After toluene was removed, the residue was washed with sodium bicarbonate and distilled water, followed by extracting with ethyl acetate. AD was purified by com-pletely removing ethyl acetate. The synthesis scheme is shown in Figure1. The chemical structure of the synthe-sized AD and starting chemicals was characterized by Fourier transform-infrared (FT-IR) spectroscopy and nuclear magnetic resonance (NMR) spectroscopy. The proton NMR (1HNMR) spectra were obtained on a 500 MHz Bruker NMR spectrometer (Bruker Avance II, Bruker BioSpin Corporation, Billerica, MA) using deuter- ated dimethyl sulfoxide and chloroform as solvents and FT-IR spectra were obtained on a FT-IR spectrometer (Mattson Research Series FT/IR 1000, Madison, WI).
Figure 1. Schematic diagram for the structures of the oli-gomers used in the study and synthesis of AD from the re-action of DA with AC.
2.3. Preparation of Specimens
The antibacterial resin composite was prepared as de-scribed previously . Briefly, the composite was for-mulated with a two-component system (liquid and pow-der). The liquid was formulated with CQ (photo-initiator, 1% by weight), DMAEMA (activator, 2%), AD, Bis-GMA, UDMA and BisEMA, where AD/a mixture (BisGMA/UDMA/BisEMA = 1:1:1, by weight) = 0%, 5%, 10%, 20%, 30%, 40%, 50% and 70% (by weight). The schematic structures of BisGMA, BisEMA and UDMA are shown in Figure1. The untreated glass pow- ders (Herculite XRV, 0.7 microns) were used as fillers and treated with γ-(trimethoxysilyl)propyl methacrylate as described else- where . A filler level at 75% (by weight) was used throughout the study. After mixing, the composite was filled into glass tubing to form a cylindri-cal specimen (4 mm in diameter by 8 mm in length) for CS and a disk- shape specimen (4 mm in diameter by 2 mm in depth) for antibacterial tests. Specimens were ex-posed to blue light (EXAKT 520 Blue Light Polymeriza-tion Unit, EXACT Technologies, Oklahoma City, OK, USA) for 2 min.
2.4. Strength and Viscosity Measurement
The CS test was performed on a screw-driven mechani-cal tester (QTest QT/10, MTS Systems Corporation, Eden Prairie, MN, USA) with a crosshead speed of 1 mm/min. The sample sizes were n = 6 - 8 for each for-mulation. CS was calculated using an equation of CS = P/πr2, where P = the load at fracture and r = the radius of the cylinder. The viscosity of the formulated liquid was determined at 23˚C using a cone/plate viscometer (RVDV- II+CP, Brookfield Eng. Lab. Inc., MA, USA), as de-scribed elsewhere .
2.5. Antibacterial Test
The antibacterial test was conducted following the pub-lished procedures . S. mutans was used to evaluate the antibacterial activity of the studied composites. Briefly, colonies of S. mutans were suspended in 5 mL of tryptic soy broth (TSB), supplemented with 1% sucrose, to make a suspension with 108 CFU/mL of S. mutans, after 24 h incubation. Specimens pretreated with ethanol (10 s) were incubated with S. mutans in TSB at 37˚C for 48 h under 5% CO2. After equal volumes of the red and the green dyes (LIVE/DEAD BacLight bacterial viability kit L7007, Molecular Probes, Inc., Eugene, OR, USA) were combined in a microfuge tube and mixed thoroughly for 1 min, 3 μL of the dye mixture was added to 1 mL of the bacteria suspension, mixed by vortexing for 10 s, soni-cating for 10 s as well as vortexing for another 10 s, and kept in dark for about 15 min, prior to analysis. Then 20
us-ing a fluorescent microscope (Nikon Microphot-FXA, Melville, NY, USA). Triple replica was used to obtain a mean value for each material. For evaluation of the saliva effect, human saliva (obtained from a healthy volunteer) was centrifuged for 15 min at 12,000 g to remove debris . After the supernatant was filtered with a 0.45 μm sterile filter, the filtrate was stored in a freezer (–20˚C) prior to testing. The sterilized composite specimen was incubated in a small tube containing 1 ml of saliva at 37 oC for 2 h , followed by placing in 5 ml TSB sup-plemented with 1% sucrose. The rest of the procedures were the same as above.
2.6. Aging of the Specimens
The specimens for both CS and antibacterial activity ag-ing tests were conditioned in distilled water at 37˚C for 1 day, 3 days and 7 days, followed by direct testing for CS (see 2.4) and incubating with S. mutans for 48 h for anti-bacterial testing (see 2.5).
2.7. Statistical Analysis
One-way analysis of variance (ANOVA) with the post hoc Tukey-Kramer multiple-range test was used to de-termine significant differences of both CS and antibacte-rial tests among the mateantibacte-rials in each group. A level of α = 0.05 was used for statistical significance.
3. Results and Discussion
Furanone-containing materials are reported to have a broad range of biological and physiological properties including antitumor, antibiotic, haemorrhagic and insec-ticidal activity [23-26]. The biological mechanism of these derivatives is still under investigation . To ex-
plore the application of these compounds in dental re- search, we synthesized a photocurable furanone deriva-tive and applied it to dental resin composites.
Table 1 shows characteristic peaks for DA, AC and
AD from both FT-IR and 1HNMR spectra. For FT-IR, the disappearance of the peak at 3362 for pseudo hy-droxyl group on DA and appearance of the new peaks at 1807, 1764, 1500, 804 and 670 for both carbonyl and C=C groups on acrylate confirmed the formation of AD. For 1HNMR, the disappearance of the chemical shift at 3.45 (-OH) and all the chemical shifts towards a high field confirmed the formation of AD.
Figure2 shows the effect of the AD content on CS
and S. mutans viability of the experimental composite. For CS, the AD addition did not change the CS of the composite until reaching 40%. From 40% to 70%, CS decreased 11% - 27% of its original value. For the S. mutans viability, increasing the AD content significantly decreased the S. mutans viability. The mean viability values were from 82 to 1% with 5 to 70% AD addition, where all the values were significantly different from each other (p < 0.05). The result indicates that this new furanone derivative has potent antibacterial activity. In addition, if we incorporate it within 30% - 40%, the CS of the resin composite can be kept nearly unchanged. During the course of study, we also found that the vis-cosity (154 cp) of AD was similar to that (132 cp) of TEGDMA. Therefore we decided to use AD to replace TEGDMA (a major component currently used in most commercial resin composites), to avoid a significant change in viscosity and possibly subsequent changes in other properties. The formulation with 30% AD addition in a mixture of BisGMA, BisEMA and UDMA showed a viscosity of 384 (cp), which is similar to that (345 cp) for the BisGMA/TEGDMA (50/50) mixture (a formulation
Table 1. The characteristic peaks from FT-IR and 1HNMR spectra.
Material The characteristic peaks from FT-IR or 1HNMR
The characteristic peaks (cm–1) from FT-IR
3362 (O-H stretching on -OH), 1766 (C=O stretching on carbonyl group), 1644 (C=C stretching on internal C=C), 1332, 1237 and 949 (C-O-C stretching on pseudo ester), 1451, 1026 and 778 (O-H deformation on pseudo –OH), 1279, 1118, 889 and 602 (C-O stretching on pseudo C-OH), 746 (C-Cl stretching)
AC 1758 (C=O stretching on carbonyl group), 1610 (C=C stretching), 1395 and 1145 (C-H deformation on -C=C- group), 1284, 1074, 935 and 606 (C-O stretching on carbonyl group), 971 and 755 (C-H out of plane vibration on -C=C), 705 (C-Cl stretching)
1807 and 1764 (C=O stretching on carbonyl groups of both pseudo ester and acrylate), 1639 (C=C stretching on acrylate and internal C=C), 1500 (C-O-C deformation on newly formed ester), 1407 and 1137 (C-H deformation on C=C from acrylate), 1330 and 1232 (C-O-C stretching on pseudo ester), 1295, 1068, 934 and 608 (C-O stretching on carbonyl group), 985 (C-H out of plane vibration on -C=C), 889 (C-O stretching on newly formed ester), 804 and 670 (C-H vibration on newly formed C=C group), 745 (C-Cl stretching on Cl-C=C group).
The characteristic chemical shifts (ppm) from 1HNMR
DA 6.25 (-CH) and 3.45 (-OH)
AC 6.21, 6.05 and 5.82 (H2C=CH-)
AD 7.20 (-CH), 6.55, 6.30 and 6.15 (H2C=CH-)
Figure 2. Effect of the AD content on CS and the S. mutans viability of the experimental composite: AD content (%, by weight) = AD/(AD/BisGMA/UDMA/BisEMA), where BiS-GMA/UDMA/BisEMA = 1:1:1 (by weight); The filler/resin ratio = 75% (by weight). For CS, specimens were used di-rectly for the testing. For the S. mutans viability, specimens were incubated with S. mutans before antibacterial testing.
currently being used in commercial dental composites). This result might possibly help minimize shrinkage and exotherm for this new antibacterial resin composite.
Figure3 shows the effect of human saliva on the S.
mutans viability after culturing with the modified com-posite. No statistically significant differences in the S. mutans viability were found between the composites with and without human saliva treatment. It was reported that saliva can significantly reduce the antibacterial activity of the QAS or PQAS-containing materials based on the mechanism of contact inhibition [21,22]. Due to saliva coating or protein film formation on the antibacterial surface of the material, the antibacterial capability be-came less effective [21,22]. The reduction was attributed to the interaction between positive charges on QAS or PQAS and amphiphilic protein macromolecules in saliva. Unlike QAS or PQAS, AD does not carry any charges. That may be why the AD-modified resin composite did not show any reduction in antibacterial activity after treating with saliva.
Figure 4 shows the effect of the modified composite
aging in water on CS and S. mutans viability. After 7-day aging in water, all the composite specimens with AD addition showed no statistically significant differences in either CS or S. mutans viability from one another (p > 0.05). It is known that dental resin composites show a certain degree of degradation due to water sorption caused by two hydroxyl groups pendent on BisGMA and three -CH2CH2O- units on TEGDMA . The absorbed water can hydrolyze the silane bond that is used to cou-ple resin with fillers, de-bond the resin-filler interface and thus reduce the mechanical strengths with time .
Figure 3. Effect of human saliva on the S. mutans viability after culturing with the composites: The formulations were the same as those described in Figure 2. Specimens were soaked in human saliva at 37˚C for 2 h, followed by incu-bating with S. mutans before antibacterial testing.
Figure 4. Effect of aging on CS and the S. mutans viability of the experimental composite: The formulation was the same as those described in Figure 2, except for AD content = 30%. Specimens were conditioned in distilled water at 37˚C for 1, 3 and 7 days prior to testing.
of the former. The result might also imply that the AD- modified resin composite can has a long-lasting antibac-terial function, because otherwise the composite would lose its CS if AD was leachable.
Our future studies will include evaluation of other me-chanical and physical properties and biocompatibility of the experimental composite. In conclusion, we have de-veloped a novel antibacterial dental resin composite with comparable mechanical strength and long-lasting anti-bacterial function. Within the limitations of this study, the developed experimental resin composite may be clinically attractive because all dental restoratives need to be long-lasting.
This work was sponsored by NIH challenge grant (RC1) DE020614
 I. A. Mjor, J. E. Dahl and J. E. Moorhead, “Placement and Replacement of Restorations in Primary Teeth,” Acta Odontologica Scandinavica, Vol. 60, No. 1, 2002, pp. 25- 28.
 H. Forss and E. Widstrom, “Reasons for Restorative Therapy and Longevity of Restorations in Adults,” Acta Odontologica Scandinavica, Vol. 62, No. 2, 2004, pp. 82- 86.
 J. Manhart, F. Garcia-Godoy and R. Hickel, “Direct Pos- terior Restorations: Clinical Results and New Develop- ments,” Dental Clinics of North America, Vol. 46, No. 2, 2002, pp. 303-339. doi:10.1016/S0011-8532(01)00010-6  V. Deligeorgi, I. A. Mjor and N. H. Wilson, “An Over-
view of Reasons for the Placement and Replacement of Restorations,” Primary Dental Care, Vol. 8, No. 1, 2001, pp. 5-11. doi:10.1308/135576101771799335
 R. G. Craig and J. M. Power, “Restorative Dental Materi- als,” 11th Edition, Mosby-Year Book Inc., St Louis, 2002.
 A. Wiegand, W. Buchalla and T. Attin, “Review on Fluo- ride-Releasing Restorative Materials—Fluoride Release and Uptake Characteristics, Antibacterial Activity and In- fluence on Caries Formation,” Dental Materials, Vol. 23, No. 3, 2007, pp. 343-362.
 P. W. Osinaga, R. H. Grande, R. Y. Ballester, M. R. Simionato, C. R. D. Rodrigues and A. Muench, “Zinc Sul- fate Addition to Glass-Ionomer-Based Cements: Influ- ence on Physical and Antibacterial Properties, Zinc and Fluoride Release,” Dental Materials, Vol. 19, No. 3, 2003, pp. 212-217. doi:10.1016/S0109-5641(02)00032-5  Y. Takahashi, S. Imazato, A. V. Kaneshiro, S. Ebisu, J. E.
Frencken, F. R. Tay, “Antibacterial Effects and Physical Properties of Glass-Ionomer Cements Containing Chlor-
hexidine for the ART Approach,” Dental Materials, Vol. 22, No. 7, 2006, pp. 467-452.
 K. Yamamoto, S. Ohashi, M. Aono, T. Kokubo, I. Ya- mada and J. Yamauchi, “Antibacterial Activity of Silver Ions Implanted in SiO2 Filler on Oral Streptococci,” Dental Materials, Vol. 12, No. 4, 1996, pp. 227-229.  T. Syafiuddin, H. Hisamitsu, T. Toko, T. Igarashi, N.
Goto, A. Fujishima and T. Miyazaki, “In Vitro Inhibition of Caries Around a Resin Composite Restoration Con- taining Antibacterial Filler,” Biomaterials, Vol. 18, No. 15, 1997, pp. 1051-1057.
 B. Gottenbos, H. C. van der Mei, F. Klatter, P. Nieuwen- huis and H. J. Busscher, “In Vitro and in Vivo Antimicro- bial Activity of Covalently Coupled Quaternary Ammo- nium Silane Coatings on Silicone Rubber,” Biomaterials, Vol. 23, No. 6, 2002, pp. 1417-1423.
 P. Thebault, E. T. de Givenchy, R. Levy, Y. Vanden- berghe, F. Guittard and S. Geribaldi, “Preparation and Antimicrobial Behaviour of Quaternary Ammonium Thiol Derivatives Able to Be Grafted on Metal Surfaces,” Euro- pean Journal of Medicinal Chemistry, Vol. 44, No. 2, 2009, pp. 717-724. doi:10.1016/j.ejmech.2008.05.007
 S. Imazato, R. R. Russell and J. F. McCabe, “Antibacte- rial Activity of MDPB Polymer Incorporated in Dental Resin,” Journal of Dentistry, Vol. 23, No. 3, 1995, pp. 177-181. doi:10.1016/0300-5712(95)93576-N
 H. Murata, “Permanent, Non-Leaching Antibacterial Sur- faces—2: How High Density Cationic Surfaces Kill Bac- terial Cells,” Biomaterials, Vol. 28, No. 32, 2007, pp. 4870-4879. doi:10.1016/j.biomaterials.2007.06.012  G. Q. Lu, D. C. Wu and R. W. Fu, “Studies on the Syn-
thesis and Antibacterial Activities of Polymeric Quarter- nary Ammonium Salts from Dimethylaminoethyl Metha- crylate,” Reactive and Functional Polymers, Vol. 67, No. 4, 2007, pp. 355-366.
 S. B. Lee, R. R. Koepsel, S. W. Morley, K. Matyjaszewski, Y. Sun and A. J. Russell, “Permanent, Nonleaching An- tibacterial Surfaces. 1. Synthesis by Atom Transfer Radi- cal Polymerization,” Biomacromolecules, Vol. 5, No. 3, 2004, pp. 877-882. doi:10.1021/bm034352k
 F. Li, Z. G. Chai, M. N. Sun, F. Wang, S. Ma, L. Zhang, M. Fang and J. H. Chen, “Anti-Biofilm Effect of Dental Adhesive with Cationic Monomer,” Journal of Dental Research, Vol. 88, No. 4, 2009, pp. 372-376.
 F. Li, J. Chen, Z. Chai, L. Zhang, Y. Xiao, M. Fang and S. Ma, “Effects of a Dental Adhesive Incorporating Anti- bacterial Monomer on the Growth, Adherence and Mem- brane Integrity of Streptococcus mutans,” Journal of Den- tistry, Vol. 37, No. 4, 2009, pp. 289-296.
rials, Vol. 27, No. 21, 2006, pp. 3995-4002. doi:10.1016/j.biomaterials.2006.03.003
 Y. Weng, X. Guo, V. J. Chong, L. Howard, R. L. Gregory and D. Xie, “Synthesis and Evaluation of a Novel Anti- bacterial Dental Resin Composite with Quaternary Am- monium Salts,” Journal of Biomechanical Science and Engineering, Vol. 4, No. 3, 2011, pp. 147-157.
 S. Imazato, N. Ebi, Y. Takahashi, T. Kaneko, S. Ebisu and R. R. B. Russell, “Antibacterial Activity of Bacteri- cide-Immobilized Filler for Resin-Based Restoratives,” Biomaterials, Vol. 24, No. 20, 2003, pp. 3605-3609. doi:10.1016/S0142-9612(03)00217-5
 N. Ebi, S. Imazato, Y. Noiri and S. Ebisu, “Inhibitory Ef- fects of Resin Composite Containing Bactericide-Immo- bilized Filler on Plaque Accumulation,” Dental Materials, Vol. 17, No. 6, 2001, pp. 485-491.
 J. H. Jung, S. Pummangura, C. Chaichantipyuth, C. Pata-rapanich, P. E. Fanwick, C. J. Chang and J. L. Mclaughlin,
“New Bioactive Heptenes from melodorum fruticosum (Annonaceae),” Tetrahedron, Vol. 46, No. 15, 1990, pp. 5043-5054. doi:10.1016/S0040-4020(01)87811-X
 E. Lattmann, S. Dunn, S. Niamsanit and N. Sattayasai, “Synthesis and Antibacterial Activities of 5-Hydroxy-4- Amino-2(5H)-Furanones,” Bioorganic & Medicinal Chem- istry Letters, Vol. 15, No. 4, 2005, pp. 919-921.
 D. Xie, M. Faddah and J.-G. Park, “Novel Amino Acid Modified Zinc Polycarboxylates for Improved Dental Cements,” Dental Materials, Vol. 21, No. 8, 2005, pp. 739-748. doi:10.1016/j.dental.2005.01.008
 J. B. Jones and J. M. Young, “Carcinogenicity of Lac- tones III: The Reactions of Unsaturated 4-Lactones with l-Cysteine,” Journal of Medicinal Chemistry, Vol. 11, No. 6, 1968, pp. 1176-1182. doi:10.1021/jm00312a017  J. L. Drummond, “Degradation, Fatigue, and Failure of
Resin Dental Composite Materials,” Journal of Dental Research, Vol. 87, No. 8, 2008, pp. 710-719.